The effects of beating, web forming and sizing on the surface energy of
kraft fibres evaluated by inverse gas chromatography
*, J.M.R.C.A. Santos2
, A.A. Martins3
and M.M. Figueiredo1
Department of Chemical Engineering, University of Coimbra, Pinhal de Marrocos, 3030-290 Coimbra, Portugal; 2Department of Chemical Technology, Polytechnic Institute of Braganc¸a, Campus de Santa Apolo´nia, 5301-857 Braganc¸a, Portugal;3RAIZ–Forest and Paper Research Institute, 3801-501 Eixo, Aveiro, Portugal; *Author for correspondence, e-mail: firstname.lastname@example.org
Received 7 April 2004; accepted in revised form 13 December 2004
Key words: Eucalyptus globulus, IGC, Kraft pulps, Paper properties, Surface energy
In this work attention has been focused on the eﬀects of papermaking beating, web forming and sizing operations on the physical/chemical surface properties of bleachedEucalyptus globuluskraft ﬁbres. Inverse gas chromatography (IGC) was used to determine the dispersive component of surface tension (csd) as well
as the acidic/basic character (according to the Lewis concept) of the solid surfaces (pulp ﬁbres and pulp handsheets). The results have shown that the main eﬀect of beating is to increase the ﬁbre’s Lewis acidic character. Web forming caused a strong decrease incsdand signiﬁcant increments in the adhesion works of
both acidic and basic probes, lowering the ratio between the two. Nevertheless, the surface of handsheets still exhibited a dominant acidic character. The sizing operation did not change the dispersive component of the surface tension signiﬁcantly but decreased the diﬀerence between the adhesion works of the acidic and basic probes, rendering the handsheet surface less Lewis acidic and more Lewis basic. Thus, although internal sizing is expected to strongly inﬂuence liquid spreading at the paper surface and liquid penetration of the ﬁbre’s network, it is concluded that beating and web forming lead to important changes in the surface energetic properties of theEucalyptus globulus kraft ﬁbres.
Abbreviations: A – molecular surface area of the probes used in the IGC study; Acet – acetone; AN* – Gutmann’s modiﬁed acceptor number; CHCl3– trichloromethane; DCM – dichloromethane;DN –
Gut-mann’s donor number; EtAcet – ethyl acetate;F– carrier gas ﬂow rate (measured with a digital ﬂow meter); GC – gas chromatography; IGC – inverse gas chromatography; J – correction factor for gas compress-ibility;Ka– surface Lewis acidity;Kb– surface Lewis basicity;N– Avogadro’s constant;R– ideal gas law constant;T– temperature in Kelvin;t0– retention time of the non-interacting molecule;tr– retention time of the probe molecule; THF – tetrahydrofuran;Vn– net retention volume;DG– free energy of adsorption of the probe on the stationary phase surface;DGd– dispersive component of the free energy of adsorption;
DGs– speciﬁc component of the free energy of adsorption;DHs– enthalpy of adsorption;DSs– entropy of adsorption;cld– dispersive component of the surface free energy of the liquid;csd– dispersive component of
the surface free energy of the solid; csp – polar component of the surface free energy of the solid;Was–
Eucalypt ﬁbres are being used worldwide to pro-duce the highest quality printing and writing paper grades. This is due, ﬁrstly, to the characteristics of the eucalypt ﬁbre itself. Compared to the most commonly used hardwood ﬁbres, in general euca-lypt ﬁbres exhibit lower ﬁbre length and width but similar wall thickness, which leads to a higher number of ﬁbres per unit mass and a unique combination of stiﬀness and conformability capacity upon beating. These features provide the paper with high opacity, high bulk, excellent for-mation, excellent surface smoothness and enough strength, for good runability and superior end usage performance. However, it is well known that the speciﬁc conditions of pulp production (cooking and bleaching) aﬀect the internal and the surface chemical composition of the ﬁbres, which is of consequence to the surface, structural, optical and strength properties of the papersheet. Further-more, the papermaking operations of beating, web forming and sizing play an important role in the ﬁnal quality of the paper. The beating operation (a mechanical process in which ﬁbres undergo high shear and compression forces in the presence of water) aims at improving bonding properties, which decreases the pulp drainability, the paper porosity and optical properties and increases the paper mechanical resistance. Furthermore, in or-der to enhance paper resistance to liquid penetra-tion, chemical sizers like AKD (alkyl ketene dimer) are added to the stock.
Among other factors, diﬀerences in the surface energy determine changes in the surface adhesive properties and spreading of liquids (like inks) as well as changes in their penetration into the ﬁbres network. Since the ﬁbre surface properties can inﬂuence the ﬁnal product quality, it is not sur-prising that a large amount of research work is being carried out on the study of the surface energetic characteristics of papermaking cellulose ﬁbres and the interaction of these surfaces with other systems, such as printing inks (Banerjee 1991; Santos et al. 2001). Adhesion between these systems is directly related to their capability to interact by means of dispersive and acid–base in-termolecular interactions. Therefore, the charac-terisation of these phenomena is of major importance.
In what concerns eucalypt ﬁbres, studies have been undertaken to investigate the eﬀects of cooking and bleaching conditions on the surface and strength properties of the corresponding kraft pulps (Shen and Parker 1999; Aquino et al. 2002). The study of Aquino et al. (2002) on Eucalyptus globulus kraft ﬁbres has revealed that these prop-erties are highly dependent on the history of the cooking and bleaching processes. For instance, high cooking temperatures strongly decrease the ﬁbre surface free energy and the introduction of an oxygen deligniﬁcation stage prior to bleaching enhances the Lewis acidic character of the ﬁbres. However, the eﬀect of subsequent papermaking operations, like beating and web forming, on the ﬁbre’s surface energy properties is not yet well known.With regard to the eﬀects of AKD sizing, the work of Shen et al. (1998) and that of Lee and Luner (1989) are worth mentioning.
The purpose of the present study is to examine changes in the surface energy of ﬁbres due to beating and sizing operations. Comparisons are also made between ﬁbre surface free energy of pulp and of handsheets in order to investigate the eﬀects of ﬁbre bonding and collapse, and migration of ﬁnes that occur at the web formation stage. The present work is part of a more extensive work whose main objective is to study the relationship between chemical and physical properties of ﬁbres and ﬁbre networks and the functional properties of the paper, in order to assess the contribution of these relationships to the printing performance of oﬃce papers.
Moreover, IGC has been increasingly used to characterize the surface thermodynamic properties of many inorganic and organic materials, like polymers, pigments, coatings, wood meal, wood pulp, paper, etc. (Al Saigh 1994; Papirer and Ba-lard 1999; Santos et al. 2001; 2002a,b). More information on theoretical and practical aspects of this technique can be found in reviews such as that of Papirer and Balard (1999) and that of Al Saigh (1994).
The IGC technique enables the evaluation of several surface energy related parameters, namely the dispersive component of the surface tension, arising from London and Van-der-Waals forces, and the acid/base character according to the Lewis concept (i.e., ability to accept and donate elec-trons). IGC is very similar to conventional gas chromatography (GC), the main diﬀerence being the fact that the material under study is the sta-tionary phase introduced into the chromato-graphic column, whereas the compounds injected (probes) have well-known properties. As men-tioned above, in this work, the packed materials under investigation are pulp and pulp handsheets.
Materials and methods
Eucalyptus globulus pulp was produced in a 7 l laboratory MK digester (model 409 MII from M/ K Systems, Inc.) by the kraft process. The cooking conditions were 160 C cooking temperature
dur-ing 45 min, 1 C/min heating rate, a liquor to
wood ratio of 4, 16% active alkali charge, as Na2O, and 30% sulphidity, resulting in a kappa
number of 14.8. The pulp was then bleached by applying a DEDED sequence to achieve a brightness of 90% ISO (sample A). In order to analyse the changes on the surface free energy due to the beating process, a portion of the bleached
pulp was beaten in a laboratory PFI mill to achieve 30 Schopper Riegler (sample B). To study the inﬂuence of sheet formation and sizing on the surface characteristics of ﬁbres, handsheets were made (according to ISO 5269/1-1979) using the beaten pulp with and without the sizing agent AKD, samples D and C, respectively. The sizing agent emulsion (with 13.5% active component supplied by RAISIO Chemicals Ltd.) was added to the pulp suspension after addition of sodium hydrogen carbonate (0.1%), which is the reaction catalyst. After strong mixing, laboratory round sheets were formed and subjected to drying (for AKD curing) during 10 min at 80C. The AKD
amount was adjusted to obtain 180 s HST (Her-cules Sizing Test) level. Table 1 summarises the characteristics of the several samples tested.
Inverse gas chromatography
A Perkin Elmer 8410 gas chromatograph equipped with a hydrogen ﬂame ionization detector (FID) was used for IGC data collection. The instrument was connected to a Kompensograph Siemens integrator. Stainless steel columns, 0.5 m long and 0.4 mm ID, were degreased, washed and dried before packing. In order to reduce the particles size, samples A and B were milled and samples C and D were cut into small pieces (about 2 mm·2 mm). On average, approximately 1.3 g of
milled pulp and 2 g of handsheet pieces were packed into the GC columns using a vacuum pump. The packed columns were conditioned overnight at 105C under a helium ﬂow before
any measurements were made. This procedure aims to remove any volatiles, including water molecules, that may be adsorbed at the stationary phase surface and that, consequently, could aﬀect the retention of the probe molecules. As all the columns are subject to the same pre-treatment conditions, this procedure is not expected to
Table 1. Summary of sample characteristics.
Sample A Sample B Sample C Sample D
Sample type Pulp Pulp Handsheet Handsheet
PFI rpm to 30 SR 1200 1200 1200
Grammage (g/m2) 80 80
contribute to the observed diﬀerences in the sur-face energy of the samples analysed.
Experiments were carried out at column tem-peratures between 40 and 60 C, at 5C intervals,
in order to evaluate the variation of csd with
temperature as well as the enthalpies of adsorption for the polar probes. The injector and detector were kept at 180 and 200 C, respectively. Helium
was used as carrier gas and its ﬂow was selected to ensure that neither absorption nor diﬀusion of the probes would occur inside the column stationary phase. Minute quantities of probe vapour (<1ll)
were injected into the carrier gas ﬂow to ensure that the experiments took place at inﬁnite dilution. The probes were of chromatographic grade and used as received (Sigma–Aldrich Ltd.). Their re-levant properties are listed in Table 2. The results reported for the work of adhesion of acidic and basic probes were estimated from the retention times obtained for tetrahydrofuran (basic probe) and chloroform (acidic probe). Replicated mea-surements were performed with two columns pre-pared in the same way. Retention times were the average of at least ﬁve injections. Reproducibility between runs was always better than 2%. The retention times were determined graphically according to the Conder and Young method (Kamdem and Riedl 1992).
Natural gas with 83.7% methane was used to determine the dead retention volume. It was en-sured that no extraneous peaks were obtained due to the use of natural gas, the methane peak being clearly identiﬁed, and peaks relating to other components being not signiﬁcant (as expected, as the runs were carried out under inﬁnite dilution conditions).
IGC data analysis
IGC data processing was carried out according to customary methods, well described in the literature
(see for instance Chtourou et al. (1995)). In IGC, an inert carrier gas elutes a minute quantity of a probe molecule through a column packed with the mate-rial under study. Due to the interactions between the two phases, the probe molecules are retained for a certain time,tr, which is used to calculate the net retention volume,Vn, according to Eq. (1):
Vn ¼ ðtrt0ÞFJ: ð1Þ
Here t0 is the dead retention time of the marker probe,Fis the carrier gas ﬂow rate (measured with a digital ﬂow meter) andJis the correction factor for gas compressibility (Belgacem et al. 1995).
Determination of the dispersive component of surface tension
Assuming that experiments take place at inﬁnite dilution, the free energy of adsorption of the probe on the stationary phase surface per mole,DG, can be determined from the retention volume, Vn, according to
DG¼ RTlnðVnÞ þC1: ð2Þ
HereRis the ideal gas constant,Tis the absolute column temperature and C1 is a constant that depends upon the chromatographic column and the reference state (Dorris and Gray 1980). Consider-ing that the dispersive and speciﬁc components, respectivelyDGdandDGs, are additive, as suggested by Fowkes (1987), Eq. (2) can be rewritten as
DGdþDGs¼ RTlnðVnÞ þC1: ð3Þ
On the other hand, the free energy of adsorption can be related to adhesion work, Wa (Dorris and Gray 1980), according to
Here N is Avogadro’s number and A the cross-sectional area of the probe to be tested (Table 2). If non-polar components (such as n-alkanes) are
Table 2. Characteristics of IGC probes (Kamdem et al. 1993; Santos et al. 2001).
Polar probes A(A˚2) cl d
(mJ/m2) ANa(kJ/mol) DN(kJ/mol) Alkanes A(A˚2) cl d
CHCl3a 44.0 25.0 22.6 – C6H14 51.4 18.4
DCMa 31.5 27.6 16.3 – C
7H16 57.0 20.3
THFa 45.0 22.5 2.1 84.2 C
8H18 62.8 21.3
EtAceta 48.0 19.6 6.3 71.7 C
9H20 68.9 22.7
C10H22 75.0 23.9
used, only dispersive interactions occur and the adhesion work is given by
Here csdandcldare the dispersive components of
the surface tension of the solid (stationary phase) and of the liquid, respectively.
Replacing Eqs. (4) and (5) in Eq. (2) leads to
The slope of the straight line, referred to as the reference line, obtained by plotting RTln(Vn) vs. 2N(cld)1/2A, for a homologous n-alkane series
(Figure 1(a)), leads to the determination of csdfor
a given temperature.
Determination of the surface acid–base properties
Acid–base characteristics of ﬁbre surface are determined by analysing the interaction of the polar probes with the solid surface and quantifying the deviation from the reference line, leading to the estimation of the speciﬁc free energy,DGs, as
DGs¼RTlnðVnÞ RTlnðVn;refÞ: ð7Þ
Here Vn,ref is the retention volume established by then-alkanes reference line (Eq. (1)),Vnbeing now the retention volume of the polar probes. This calculation is also illustrated in Figure 1(a).
The adhesion work between the polar probes tested and the ﬁbres, Was, can be evaluated from the speciﬁc free energy, given by Eq. (7), as
By carrying out experiments at diﬀerent tem-peratures, it is possible to determine the enthalpy and entropy of adsorption, respectively DHs and
DSs, from the plots ofDGs=Tvs. 1/T, according to the following equation:
DHs T DS
The acidic and basic constants, Ka and Kb, respectively, are calculated using Eq. (10) from the linear relationship DHs/AN* vs. DN/AN* for the
series of polar probes tested, characterized by diﬀerentAN* (modiﬁed acceptor) andDN(donor) numbers (Table 2). The procedure is illustrated in Figure 1(b).
AN ¼Ka DN
The retention times obtained from the IGC experiments are converted in net retention vol-umes, according to Eq. (1). For subsequent data reduction the net retention volume can be nor-malized by using the stationary phase surface area or mass (the latter being the rule). In any case, and bearing in mind the data reduction mathematical procedures, it should be noted that the normali-zation of the net retention volume, using either the stationary phase mass or surface area, does not inﬂuence the values of csd or its variation with
temperature (dcsd/dT), nor the values ofWas,DHs, KaandKb.
The limitations of the IGC are well described in the literature, and have actually been the subject of discussion in a paper published by one of the authors (Santos et al. 2002a). The best
Figure 1. Determination of (a)cs d
approach to assess the surface energetic proper-ties (surface tension, surface Lewis acidic/basic properties) of a material by IGC is the side-by-side analysis of the energy of adsorption, enthalpy of adsorption and surface Lewis acidity and basicity constants. This procedure allows for a coherent and systematic interpretation of the IGC results, leading to a more complete analysis than the sole analysis of the semi-empirical val-ues of Ka and Kb. This was the procedure adopted in the present paper.
BET surface area determination
The BET speciﬁc surface area of the IGC column stationary phases was determined by nitrogen adsorption in a Micromeritics ASAP 2000 unit.
SEM images of the IGC column stationary phases were obtained in a JEOL JSM-5310 unit, using an accelerating voltage of 10 kV.
FTIR spectra of the IGC column stationary pha-ses was carried out in a Nicolet Magma IR TM750 unit (ATR MKII Golden Gate).
Contact angle measurement
An OCA20 Dataphysics unit was used for the determination of static contact angles relating to the handsheets. The liquids used were water, formamide, diodomethane, ethylene glycol and propylene glycol. The values of contact angle were processed according to the Owens, Wendt, Rabel and Kaelble approach (OWRK method).
Results and discussion
BET surface area determination
In Table 3 are summarised the results concerning the determination of the speciﬁc surface area of the IGC column stationary phases.
In Table 3 it can be observed that the beating process applied to pulp A (production of sample B) increases the speciﬁc surface area due to the more open structure and the production of ﬁbrils along the ﬁbre’s surface. Moreover, the speciﬁc surface area of the handsheet stationary phases (samples C and D) is lower than that of the pulp samples (A and B), as expected. The stationary phase corresponding to the sized handsheet (sam-ple D) has a lower speciﬁc surface area than that of the non-sized handsheet (sample C). This may be due to reduction in porosity caused by covalent bonding between the AKD molecules and the ﬁbres and ﬁnes surface.
SEM images of the IGC columns stationary pha-ses are presented in Figures 2–5, concerning sam-ples A, B, C and D, respectively.
As mentioned, samples A and B consist of milled pulp. The milling operation aimed at reducing the size of pulp ﬂocks so that the IGC column stationary phase could be packed. It can be observed in Figures 2 and 3 that the eﬀects of this procedure do not dominate over the eﬀect of the PFI beating process (which results in a more open structure and the production of ﬁbrils along the ﬁbre’s surface). This is further supported by the fact that even after the milling procedure sample B has a greater surface area than sample A (Table 3). The consequences of the pulp mill-ing, if this operation had been extended, would be increased exposure of the cross sectional sur-face and lumen sursur-face in addition to the detachment of ﬁbre wall fragments. Conse-quently, the thermodynamic properties (csd, dcsd/
dT, Wa(THF), Wa(CHCl3), Ka and Kb) would
reﬂect this varied composition and not that of the original pulp because the milled pulp surface is expected to be richer in cellulose and hemicellu-lose. Nevertheless, the above phenomena did not
Table 3. BET surface area (m2/g) of the IGC columns sta-tionary phases.
Sample A Sample B Sample C Sample D
occur in the studied samples because of the gentle milling.
In addition, morphological diﬀerences are observed between sample B (beaten and milled pulp) and samples C and D (paper sheets made from beaten pulp), in particular the collapse of
the surface ﬁbre’s and the presence of ﬁnes and colloidal material at the ﬁbre’s surface, due to the web-forming operation. The eﬀects of these phenomena on the surface energetic properties will be discussed in detail further in this article.
Figure 4. SEM images of the IGC stationary phase relating to sample C, at magniﬁcation levels of 750·(on the left) and 3500·(on
Figure 3. SEM images of the IGC stationary phase relating to sample B, at magniﬁcation levels of 750·(on the left) and 3500·(on
Figure 2. SEM images of the IGC stationary phase relating to sample A, at magniﬁcation levels of 750·(on the left) and 3500·(on
Inverse gas chromatography
The elution peaks obtained were generally sym-metrical. For probe molecules that adsorb strongly on the stationary phase, such as THF, a tail was detected in the elution peak that did not inﬂuence the symmetry of the peak signiﬁcantly as the magnitude of the tail was prominently lower than that of the elution peak. The presence of an asymmetrical peak would be due to the existence of dead volumes inside the IGC column or to signiﬁcant surface energetic heterogeneity. In that situation, in order to account for the distribution of acidic/basic sites of various strengths, IGC un-der ﬁnite dilution conditions would be necessary. The Gaussian peaks observed indicate that the energetic heterogeneity is not signiﬁcant, for any of the samples studied, under the operation con-ditions used for the IGC study. It should be mentioned that IGC carried out under inﬁnite dilution conditions is more sensitive to the higher energy sites. IR spectroscopy was used in order to detect any contamination of the samples. No extraneous peaks, related with contaminants, were detected.
The retention times were not extrapolated to peaks of zero area as the volume of molecular probe injected in the IGC columns was residual and the IGC unit was set to the limit of probe
detection by the FID detector. Typically, the syr-inge was ﬁlled with 1ll of gaseous probe, ﬂushed
with air about 10 times, in order to ensure the creation of a Henry’s inﬁnite dilution region, and injected manually.
Determination of the dispersive component of the surface tension
The dispersive component of the surface tension,
csdat 40C, determined according to Eq. (6), and
its variation with temperature (dcsd/dT), are
pre-sented in Table 4. Figure 6 illustrates the depen-dence of csd on temperature, for all the samples
Although the modiﬁcations to which pulp A was subjected (beating, handsheet formation and siz-ing) greatly aﬀect the sample surface energetic properties, all the values obtained for csd are
consistent with those published in the literature for this type of materials (Belgacem 2000). A Whil-elmy balance was used in an attempt to determine the contact angles for the ﬁbres, but, due to their small length, it was not possible to prepare sam-ples such that reliable results could be obtained. With regard to the handsheets, the sessile droplet method was used but the size of the pores, roughness and hydrophilicity of the surface did not allow for accurate results to be obtained in the
Figure 5. SEM images of the IGC stationary phase relating to sample D, at magniﬁcation levels of 750·(on the left) and 3500·(on the right).
Table 4. Dispersive component of surface tension,csd, and its variation with temperature for all the samples tested.
Sample A Sample B Sample C Sample D
csd(mJ/m2), 40C 45.0±0.38,r2= 0.995 48.2±0.48,r2= 0.998 31.3±0.02,r2= 1.000 33.4±0.04,r2= 0.999
case of samples A, B and C. For sample D a value of 33.9 mJ/m2 for csd and of 0.3 mJ/m2 for csp
were determined. Thus, the values ofcsdfor sample
D, obtained using IGC and the sessile droplet method, are in good agreement.
The increased exposed surface area, due to the production of ﬁbrils and to the more open struc-ture formed upon beating of the pulp (samples A and B), is thought to result in increments in the amount of hydroxyl and carboxyl groups accessi-ble at the surface and, thus, of bonding sites available for interaction with the IGC molecular probes. Consequently, the surface ability to establish dispersive interactions increases (higher
csd). The dependence of csd on temperature
(Figure 6) also increases for pulp B, denoting a higher entropic contribution to the surface free energy, a consequence of the greater mobility of molecular segments, namely ﬁbrils, in the case of sample B.
The eﬀect of web forming can be examined by comparing sample B (milled pulp) and sample C (pieces of handsheet). The latter shows a much lower value of the dispersive component of surface tension and of its temperature dependence (about half). This is most probably due to the enrichment of ﬁnes and colloidal material at the surface of the handsheets. Although the milling procedure, adopted in the case of samples A and B, could inﬂuence the surface properties of the pulp, as discussed earlier (it would contribute, for example, to the higher values ofcsdobserved for samples A
and B in comparison with those observed for samples C and D), the web-forming operation is
thought to be the major cause of the diﬀerences observed upon this operation, based on the SEM images (Figures 3–5) and on the IGC results (Figure 7 and Table 5). In Figures 4 and 5, it can be clearly seen that in samples C and D the pres-ence of ﬁnes and colloidal material at the ﬁbre’s surface is very signiﬁcant and, thus, these compo-nents are expected to inﬂuence very signiﬁcantly the handsheet surface thermodynamic properties. Conversely, at the surface of the beaten pulp (sample B, Figure 3) no colloidal material can be identiﬁed (only the existence of ﬁbrils originated from the beating process).
The diﬀerences in ﬁnes and extractives concen-trations between the pulp and the handsheet ﬁbres surface have been the subject of several studies. Three types of ﬁnes have been identiﬁed: primary ﬁnes, associated with the virgin pulp, secondary ﬁnes, produced during pulp processing prior to the forming operation, and tertiary ﬁnes, produced during the ﬂow of non-retained stock around the paper machine white water system (Truong et al. 2003). Shen et al. (1998) and Truong et al. (2003) state that residual lignin and extractives of the ﬁnes fraction are present in a higher concentration (at the surface as well as in the bulk) than they are in the ﬁbres fraction. Furthermore, the concen-trations of lignin and residual extractives on the surface of the ﬁbres are not the same as those in the bulk of the ﬁbres, due to migration, resorption and reprecipitation phenomena (Shen and Parker 1999), during the cooking (Suurnakki et al. 1996) and the washing processes (Shen et al. 1998). Shen et al. (1998) have determined that the dispersive
Figure 7. Speciﬁc component of the adhesion works for the basic (THF) and the acidic (CHCl3) probes on the surfaces of samples A, B, C and D, at 40C.
component of the surface tension of the eucalypt ﬁnes is lower than that of the whole pulp (34.7 and 38.4 mJ/m2, respectively). In another study, Shen and Parker (1999) found the values of 56.6 and 48.2 mJ/m2 for cellulose and lignin, respectively. Other researchers have also found that lignin has a lowercsdthan cellulose (Belgacem 2000, Belgacem
et al. 1995). Thus, it is concluded that the decrease observed in csd when the pulp is converted to
handsheets is due to reprecipitation/migration of ﬁnes and colloidal material to the surface of the handsheet. This phenomenon would be caused by water ﬂow during the web-forming process.
Regarding the inﬂuence of sizing, expressed by the diﬀerences between the results obtained for samples C and D, no signiﬁcant change was de-tected for the surface free energy, despite other authors having reported a decrease in this parameter with sizing (Shen et al. 1998; Belgacem 2000). Possible explanations for this lack of liter-ature agreement are the diﬀerences in both the type of sizing agent and procedure and the fact that, in this work, the eﬀect of sizing was evaluated in handsheets instead of pulp ﬁbres. Thus, the ef-fect of sizing could be masked by the eﬀect of web forming.
Although the discussion that follows is mainly based on the results obtained for THF (as a model basic probe) and CHCl3(as a model acidic probe),
the acidic/basic character of the samples was evaluated using all the polar probes referred to in Table 2, the results being consistent.
In Figure 7 are presented the values obtained for the speciﬁc component of the adhesion works of THF and of CHCl3 on the surface of all the
samples analysed (derived from Eq. (8)). The val-ues obtained for the speciﬁc component of the enthalpy of adsorption of THF and of CHCl3
(derived from Eq. (9)), and the values obtained for
KaandKb(calculated from Eq. (10)) are coherent with the tendencies observed in Figure 7. The rel-ative values found for the speciﬁc component of the adhesion works and of the enthalpy of adsorption of THF and of CHCl3, as well as the
relative values found for the acidic and basic constants (Ka and Kb, respectively) are presented in Table 5.
From the results presented in Table 5, namely the ratioKa/Kb, it can be concluded that, excluding sample D, all the samples have a predominant acidic character which decreases in the following order:
sample B>sample A>sample C>sample D.
This tendency is corroborated by the values of the
Was(THF)/Was(CHCl3) and DHs (THF)/ DHs(CHCl3) ratios, revealing a good qualitative
correlation between the three approaches.
From IGC experiments Shen et al. (1998) have shown that eucalypt pulp ﬁbres are Lewis amphoteric with a strong acidic character. Our results are, thus, in agreement with expectation bearing in mind reports in literature and also the nature of cellulosic materials (extensive presence of OH and COOH functional groups).
As far as the beating eﬀect is concerned, the increased OH and COOH groups concentration at the ﬁbre’s surface in the case of sample B (a con-sequence of the beating action as discussed above) results in increased works of adhesion with the polar probes, namely with the basic probe (thus reﬂecting a signiﬁcant increase in the Lewis acidic character), Figure 7. The latter eﬀect is also clear in Table 5. Here it can be observed that the pres-ence of acidic sites relative to that of basic sites increases upon the beating operation.
As mentioned previously, the diﬀerences in surface energy upon web forming are thought to be due mainly to the increase in surface ﬁnes and colloidal material concentration. The primary ﬁnes have been shown to have a strong basic character,
Table 5. Ratios between the adhesion works (Was) and enthalpies of adsorption (DHs) of tetrahydrofuran and chloroform, and between the acidic and basic constants (KaandKb, respectively), relating to samples A, B, C and D.
Sample A Sample B Sample C Sample D
Was(THF)/Was(CHCl3), 40C 8.7 11.4 5.4 2.0
3) 17.5 21.6 4.1 2.7
in an order of magnitude similar to that of cellu-lose (Shen and Parker 1999; Shen et al. 1998). On the other hand, lignin has a lower acidity than cellulose. In addition, Shen and Parker (1999) and Belgacem et al. (1995), showed that extraction of eucalypt ﬁbres causes an increase of the works of adhesion with both acidic and basic probes. Our results (Figure 7, samples B and C), however, show that web forming increases the works of adhesion of both acidic and basic probes despite decreasing the relative acidity of the surface (Ta-ble 5). The greater concentration of ﬁnes observed in sample C (when compared to sample B) con-tributes indeed to the increase of the work of adhesion of the acidic probe (and to the decrease of the surface relative acidity). The discrepancy related to the basic probe may be justiﬁed by (1) the fact that lignin and extractives are not the only constituents of ﬁnes and colloidal material that also comprises carbohydrates, (2) the greater density of COOH and OH groups in the case of the ﬁnes and (3) the preferential orientation of these groups at the handsheet surface due to the web-forming operation conditions (towards the cellulosic surface used to absorb the water and to form the paper handsheet).
The last factor is important in many polymeric systems, as extensively illustrated by Schreiber et al. (1993). A good example is that of PMMA ﬁlms prepared either by drying in air or by drying between plaques of diﬀerent materials. When the PMMA ﬁlm is dried in air, the methacrylate groups are oriented towards the bulk of the ﬁlm, in order to minimize the PMMA ﬁlm surface free energy (as the PMMA backbone is apolar). When the PMMA ﬁlm is formed between two plaques of greater surface free energy (in this case metallic), the methacrylate groups are preferentially orien-tated towards the PMMA ﬁlm/metallic plaque interface, thus minimizing the interface surface free energy. The result is a greater interaction capability of the PMMA ﬁlm surface through speciﬁc (Lewis acid/base) forces. In the case of our samples, the pulp, after being thoroughly washed, is dried in air. On the other hand, the web-forming operation consists of placing wet handsheets be-tween two plaques of high water absorbency pa-per, followed by application of pressure. Afterwards, the sheets are dried in air. The fact that the pulp is dried in air and the handsheet is formed between two cellulosic substrates would be
expected to lead to diﬀerences in functional groups (hydroxyl and carboxyl groups) orientation at the surface, and, in particular, to increased Lewis acidic and basic character in the case of the handsheet. This reasoning must, nevertheless, be the subject of further experimental evidence.
The ﬁnes have a much larger speciﬁc surface area than the ﬁbres and have been shown to have a much higher surface charge than the ﬁbres, on a mass basis (Truong et al. 2003). When ﬁnes are removed, the eucalypt pulps studied by Truong et al. (2003) lose an average of 50% of their surface charge. The charge of the kraft pulp ﬁbres and ﬁnes results from ionization mainly of carboxylic acid groups. The diﬀerence in COOH and OH functional groups per unit mass between the ﬁnes and the ﬁbres can be explained by diﬀerences in size. Bearing in mind the typical dimensions of the ﬁbres and of the primary ﬁnes, the surface charge of ﬁnes (and, thus, the COOH and OH functional groups concentration), can be estimated to be around 10 times that of the ﬁbres. A practical evidence is that a large amount (50–75%) of AKD sizing agent has been proven to be adsorbed by the ﬁnes in eucalypt pulps (Truong et al. 2003). Thus, the results obtained for the diﬀerences in the Lewis acid/base properties after web forming are thought to be due mainly to the higher concentration of ﬁnes (with higher charge density) in the handsheet surface.
It is clear from Figure 7 that the diﬀerences be-tween the adhesion works of the acidic and the basic probes decreased from sample C to sample D, due to sizing (that is, the surface of the sized handsheet is less Lewis acidic and more Lewis basic than the unsized sample). In addition, the ratioKa/
Figures 4 and 5), thus, decreasing opportunity for sorption and spreading of liquids.
In this work, inverse gas chromatography was used to study the inﬂuence of beating, web forming and sizing on surface free energy of bleached
Eucalyptus globulus kraft ﬁbres. Milled pulps or pieces of handsheets were used as the stationary phase.
The results have shown that beating, although increasing only slightly the dispersive component of the surface tension, greatly enhances the acidic character of the ﬁbres surface, probably due to a greater number of hydroxyl and carboxyl func-tional groups accessible at the ﬁbre’s surface. The speciﬁc surface area has increased as expected.
The process of web-forming decreases the spe-ciﬁc surface area and causes the retention of ﬁnes and colloidal material at the surface of the ﬁbres. Consequently, this operation greatly decreases the ability of forming dispersive intermolecular forces bonds, resulting in signiﬁcantly lower values for
csd. Nevertheless, the speciﬁc (acidic/basic)
inter-molecular interactions with the polar probes greatly increase, probably due to increased hy-droxyl and carboxyl functional group concentra-tion and exposure at the papersheet surface (a consequence of the greater concentration of ﬁnes and colloidal material).
Because of the basicity of AKD and also due to the strong bonds formed between this sizing agent and the ﬁbre surface, the availability of electron-accepting sites, relative to the electron donor sites, decreases and the surface of the sized handsheet becomes more Lewis basic.
Although internal sizing plays an important role in controlling liquid spreading at the paper surface and liquid penetration on the ﬁbre’s network, it is concluded that web forming is probably the papermaking operation that mostly contributes to the changes of the surface energetic properties of the cellulose ﬁbres.
Thanks are due to Sapiens Program for the re-search grant (PE044-PE/PPQ/34159/99). The
skilful work of EngaA. Aquino in IGC analysis, Engo V. Redondo in BET surface area determi-nation, EngoJ.P. Dias in SEM imaging and Enga M.J. Travassos in FTIR analysis is also acknowl-edged.
Al Saigh Z.Y. 1994. Recent advances in the characterisation of polymers and polymer blends using the inverse gas chroma-tography method. Polym. News 19: 269–279.
Aquino A.I., Ferreira P.J., Carvalho M.G., Amaral J.L. and Figueiredo M.M. 2002. Inﬂuence of cooking and bleaching conditions on the surface and paper properties ofEucalyptus globuluskraft pulps. Proceedings of the 2nd Iberoamerican Congress on Pulp and Paper Research, CD-ROM, CIADI-CYP, Sa˜o Paulo, Brasil.
Banerjee R.K. 1991. Surface characterization of paper and printability. IPPTA – Indian Pulp & Paper Technical Asso-ciation Annual General Meeting & Seminar on Develop-ments in Pulp mill and Paper Machine Clothings, New Delhi, pp. 75–90.
Belgacem M.N. 2000. Characterization of polysaccharides, lignin and other woody components by inverse gas chroma-tography: a review. Cell. Chem. Technol. 34: 357–383. Belgacem M.N., Czeremuszkin G. and Sapieha S. 1995. Surface
characterization of cellulose ﬁbres by XPS and inverse gas chromatography. Cellulose 2: 145–157.
Chtourou H., Riedl B. and Kokta B.J. 1995. Surface charac-terization of modiﬁed polyethylene pulp and wood pulp ﬁbres using XPS and inverse gas chromatography. Adhes. Sci. Technol. 9(5): 551–574.
Dorris C.M. and Gray D.G. 1980. Adsorption ofn-alkanes at zero surface coverage on cellulose paper and wood ﬁbres. J. Colloid Interface 77(35): 353–362.
Fowkes F.M. 1987. Role of acid–base interfacial bonding in adhesion. J. Adhes. Sci. Technol. 1(1): 7–14.
Kamdem D.P. and Riedl B. 1992. Inverse gas chromatography of lignicellulosic ﬁbres coated with a thermosetting polymer: use of peak maximum and Conder and Young methods. J. Colloid Interface Sci. 150: 507–516.
Kamdem D.P., Bose S.K. and Luner P. 1993. Inverse gas chromatography characterization of birch wood meal. Langmuir 9(11): 3039–3044.
Lee L.H. 1991. Relevance of the density-functional theory to acid-base interactions and adhesion in solids. In: Mittal K.L. and Anderson J. (eds), Acid–Base Interactions: Relevance to Adhesion Science and Technology. Utrecht, The Nether-lands, pp. 25–46.
Lee H.L. and Luner P. 1989. Characterisation of AKD sized papers by inverse gas chromatography. Nordic Pulp Paper Res. J. 4: 164–172.
Mukhopadhyay P. and Schreiber H.P. 1993. Inverse gas chro-matography for polymer surface characterization above and below Tg. Macromolecules 26: 6391–6396.
Santos J.M.R.C.A., Gil M.H., Portugal A. and Guthrie J.T. 2001. Characterization of the surface of a cellulosic multi-purpose oﬃce paper by inverse gas chromatography. Cellu-lose 8: 217–224.
Santos J.M.R.C.A., Fagelman K. and Guthrie J.T. 2002a. Characterisation of the surface Lewis acid/base properties of the components of pigmented, impact-modiﬁed, PC/PBT blends by inverse gas chromatography – phase separation and phase preference. J. Chromatogr. A 969(1–2): 119–132. Santos J.M.R.C.A., Fagelman K. and Guthrie J.T. 2002b.
Characterisation of the surface Lewis acid/base properties of poly(butylene terephthalate) by inverse gas chromatography. J. Chromatogr. A 969(1–2): 111–118.
Schreiber H.P. 1993. Aspects of component interactions in polymer systems. In: Akovali G. (ed.), The interfacial inter-actions in Polymeric composites. Kluwer Academic Publish-ers, The Netherlands, pp. 21–59.
Schultz J. and Lavielle L. 1989. Interfacial properties of carbon ﬁber-epoxy. In: Lloyd D.R., Ward T.C. and Schreiber H.P. (eds), Inverse Gas Chromatography, Characterization of Polymers and Other Materials. A.C.S, Washington, pp. 185– 202.
Schultz J. and Lavielle L. 1989. Interfacial properties of carbon ﬁber-epoxy. In: Lloyd D.R., Ward T.C. and Schreiber H.P. (eds), Inverse Gas Chromatography, Characterization of Polymers and Other Materials. A.C.S, Washington, pp. 185– 202.Schultz J. and Lavielle L. 1989. Interfacial properties of carbon ﬁber-epoxy. In: Lloyd D.R., Ward T.C. and Schreiber H.P. (eds), Inverse Gas Chromatography, Characterization of Polymers and Other Materials. A.C.S, Washington, pp. 185–202.
Shen W., Yao W., Li M. and Parker I.H. 1998. Characteriza-tion of eucalypt ﬁbre surface using inverse gas chromatog-raphy and X-ray photoelectron spectroscopy. Appita J. 51(2): 47–51.
Shen W. and Parker I.H. 1999. Surface composition and surface energetics of various eucalypt pulps. Cellulose 6: 41–55. Suurnakki A., Heijnesson A., Buchert J., Viikari L. and
Wes-termark U. 1996. Chemical characterisation of the surface layers of unbleached pine and birch kraft pulp ﬁbers. J. Pulp Paper Sci. 22(2): 43–47.